International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 07  July 2018
pISSN: 23950072
www.irjet.net
Electronic and Structural, properties of ZnTe using Density Functional Theory (DFT) P. Ashwini1, J. Mani2 1*Department
of Physics, Aalim Muhammed Salegh College of Engineering, Muthapudupet, 600 055, Tamil Nadu, India 2Department of Nuclear Physics, University of Madras, Chennai600 025, Tamil Nadu, India ***
Abstract  Chalcogenides like metal Telluride have been studied for many decades for solar cell application. Recently related cubic phases like ZnTe are attracting wide attention for many interesting applications such as thermoelectronics and sensors. Especially ZnTe being a narrow direct band gap (Band gap value = 1.2eV) semiconductor is recently researched a lot owing to its wide applications on electronic, optical, magnetic and thermoelectric devices. In order to understand the fundamental properties of ZnTe and its closely related compounds, we have performed accurate first principle calculations based on Density Functional Theory (DFT). We have used Tight bonding Linear MuffTin Orbital (TBLMTO) program. We have performed complete structural optimization by minimizing force as well as stress. The optimized structural parameters are found to be in good agreement with experimental values. We have analyzed electronic structure by calculating band features, site and orbital projected Density of States (DOS). In order to reproduce the experimental band gaps we used LDA (Local Density Approximation) and hybrid functional to describe its correlation effects better than usual LDA. The nature of bonding is analyzed using COHP (Crystal Orbital Hamiltonian Population) and charge density plots.
rocksalt (RS) and was discussed by J. Pellicer Porres et al., [6]. In this paper, we depict various physical and electronic properties of ZnTe compounds by using Density Functional Theory (DFT) [710]. The total energy of ZnTe is calculated using tight binding linear muffin tin orbital method (TBLMTO) [10, 11] and it has a band gap of 0.97 eV which is low when compared to experimental band gap value. So it provides a solution to minimizing the mismatch of results obtained from theoretical and experimental study. The experimental data collected from crystal open database for ZnTe electrical properties using DFT was discussed by PellicerPorres and S.K.Gupta et al., [12, 15]. From the experimental and Theoretical result it is observed that ZnTe exhibits ZB structure. Generally zinc blende (ZB) structure calculation can be explained effectively with the help of available experimental data [1618]. The elements belonging to the group of IIVI are very useful for technological applications [17, 18]. Here we have investigated the structural and electronic properties for ZnTe [19]. We hope that the present work will inspire the experimental group to invoke their knowledge in this particular field to analyze it experimentally [20]. The plan of the paper work is as follows section2 gives a description about computational method followed by a result and discussion in section3 which contains details about the structural properties, electronic band structure and COHP properties, finally the conclusion is given in section4.
Key Words: Chalcogenids, ZnTe, DFT, TBLMTO, LDA electronic properties, DOS, COHP. 1. INTRODUCTION In last decade with increase in computational power, several numerical simulations are being carried out which has made it possible to predict properties (structural, electronic and optical etc.) of solids with great accuracy [1,2]. Inspite of high complexity and defective forms, IIVI group of semiconducting materials remains as the major regime of research interest in condensed matter physics because of their wide band gap nature. The cubic ZnTe was synthesized in solid state using 900W microwave plasma method by Tawat Suriwong et al., [4]. This semiconducting materials showed a 2.6 eV wide direct band gap has a variety of applications; greenlightemitting diodes, solar cells, waveguides, modulators [38], and other optoelectronic and thermoelectronic devices, Young KT et al., [5]. The compound ZnTe is extensively studied on its wellknown structure zinc blende (ZB) and
ÂŠ 2018, IRJET

Impact Factor value: 7.211
2. COMPUTATIONAL DETAILS There are several methods to calculate structural, electronic and optical properties of compounds computationally. The density functional theory is one of the most accurate ways to reach acceptable results that helps us to envision the features and character of materials and nanostructure materials in particular [21]. The structural and electronic properties of (ZnTe) are investigated in this paper. The electronic band features of ZnTe in the ZB structure is studied using the Tight Binding Muffin Tin Orbital (TBLMTO) program [22], this program calculate the KohnSham eigenvalues within the framework of DFT [23]. In the calculations have been

ISO 9001:2008 Certified Journal

Page 2657
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 07  July 2018
pISSN: 23950072
www.irjet.net
performed with the use of local density approximation (LDA) [24, 25], this is includes the Coulomb interaction in the LDA Hamiltonian. The interaction between electrons and atomic cores is described by the nonnorm conserving pseudopotentials are implemented in the LMTO code [26]. The pseudopotentials are generated in accordance to the linear fixed based methods [27]. The values of the parameters U and J required for the LDA studies were found from band structure calculations for different values of U by adjusting the position of Zn3d bands to the experimentally compared band gap values [28].The Muffin Tin approximation makes it easier to solve the Schrödinger equation by the approximation potential [28,29]. In the TBLMTO program the inputs are the crystal structure while outputs are total energy, chargeand spinself consistent band structure, partial densities of states, Fermi surface, full charge and spin density plots, and partial pressures etc [3033]. In this work using in this program we have calculated the total energy, band structure, total and partial densities of states and COHP of a ZnTe material.
3.1. STRUCTURAL PROPERTIES 3.1.1. KPoint Optimization The Kpoint energy of the system is minimized and does not change anymore and appropriate for the calculation of physical properties of the given material. The calculated kpoint energy values are 17167.4634 eV. We have calculated the total energy for the Kpoint grids starting from 2 x 2 x 2 to 12 x 12 x 12, the Fig. 2 plot irreducible Kpoints and total energy and which shows that the total energy of a system does not vary significantly beyond 8 x 8 x 8 range. It is found that on further increasing the Kpoints, there is no change in total energy. So the Kpoint grid is considered to be an optimized Kpoint grid and it has been used to calculate the other properties of systems in our study.
3. RESULT AND DISCUSSSION This study is mainly concentrated on the group IIVI metal chalcogenides and their structural, band structures and total and partial density of states and COHP we will calculate using density functional theory (DFT). The compounds zinc telluride (ZnTe) is a stable crystalline compound formed by zinc and tellurium. The ZnTe has facecentered cubic structure in Zinc Blende (ZB) type structure with space group F43m (No: 216), (Fig.1) shows that the crystal structure of ZnTe. The initial guess crystal structural details are taken from experimental studies. We used lattice parameter of a=6.07Å with Zn and Te atoms positions is (Zn=0, 0, 0) and (Te=0.25, 0.25, 0.25), respectively.
Fig 2: Kpoint optimization Zinc Telluride (ZnTe) 3.1.2. Volume Optimization Total energy has been calculated for different volumes of crystal structure by changing the lattice parameter used in the ZB structure. The volume in which the system has the lowest total energy is said to be the ground state volume of the stable structure. The lattice parameter corresponding to the lowest energy structure is used to calculate further properties such as electronic and structural properties etc,. Fig.3 shows the calculated total energy with respect to different volumes of ZnTe. According to our calculation the ZnTe has the lowest total energy for the volume of 398 Å3. Hence the crystal structure at this volume is used for further investigation of ZnTe properties.
Fig 1: Crystal structure for ZnTe
© 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 2658
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 07  July 2018
pISSN: 23950072
www.irjet.net
contains the bands with contributions from Tes, d and Zns, d electron from Fig.5 for DOS. Second region includes more bands lying on the most occupied VB. These bands are due contributions from Tep, d and Zns, p and d contain more electrons from (Fig.5) DOS. In the unoccupied portion of the band structure a corresponding division leads to two energy regions: (i) The bottommost CB from 0 to 12 eV and (ii) Above 12 eV the one band will be appearing. There are 4 bands in region (i) with have some Zns, p; Tes, p and d electrons form Fig.5. The region (ii) the bands Znp band only most occupied in the CB above 12 eV. 3.2.2 Density of States (DOS) Fig 3: Volume of optimization for ZnTe
The important description of the electronic structure for many purposes is provided by the density of states (DOS) which is another way to visualize and analyze the electronic structure. The DOS D(E) is the number of states in the unit energy range
3.2 ELECTRONIC PROPERTIES 3.2.1 Band Structure ZnTe is seemed to be a directband gap semiconductor. A closer inspection of the energyband structure shows that the band gap is between the top of the valence band (VB) at the Gamma (G)point and the bottoms of the conduction band (CB) at the Brillouin zone (BZ) point. As the unit cell contains 46 atoms the band structure is quite interesting it is shown in Fig.4. In this band structure the energy range is from 15 to 15 eV. There is a finite energy gap at 0.97 eV between the topmostoccupied VB and the bottommost unoccupied CB. We are interested in increasing the band gap value which would be near to the experimental band gap value, so we are applied Local density Approximation (LDA). Now its band gap value (1.2 eV) increased which is near to experimental band gap value 2.26 eV [2].
⁄
( )
(
)(
⁄
)
The maximum D(E) at T=0 corresponds to the Fermi energy at the ground state, when T 0, the electrons occupy higher energy states. The Fig.5 shows the total DOS for ZnTe. Total DOS also reveals the band gap obtained in the band structure and the valence band spread which over 13 eV to 0 eV in the energy ranges. The top of the valence band has highly localized states around over the 8 eV. In the localized peak of DOS is seen in the Partial DOS in shown in the Fig.6 where the conduction Fig. 5 total density of states (DOS) for ZnTe in the Fermi line set to zero and ZnTe configurations of s, p, d states band is spread from Fermi line set as zero. The above Fermi line called conduction band and below is defined as valence band, so our convenience we shown the DOS from 0 to 15 eV range in the conduction band.
Fig 4: The electronic band structure of ZnTe. The line at 0 eV refers to Fermi energy level For the purpose of more clarity, and convenience the most occupied portion of the band structure (Fig.4) in the valence band (VB) is divided into two regions: (i). Bands lying at below 6 eV. (ii). bands lying top of the VB, and closer to Fermi Level (EF ), viz., 5 to 0 eV. Region (i)
© 2018, IRJET

Impact Factor value: 7.211
Fig 5: Total Density of States (DOS) for ZnTe in the Fermi line set to zero and ZnTe configurations of s, p, d states

ISO 9001:2008 Certified Journal

Page 2659
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 07  July 2018
pISSN: 23950072
www.irjet.net
From the partial DOS analysis, we found that the peak is due to the localization of d electrons of Zn and Te and p elections of Te. The origin of the top of the VB was mostly due to the s electron of Zn and p electron of Te which led to a further conclusion for the possibility of sp hybridization. The results show from Fig.7 covalent bonding nature as the ZnTe.
eV. Here the cubic ZnTe atoms have stronger bonding interaction with Te
Fig 7: Calculated COHP curves for ZnTe 4. CONCLUSIONS The first principle Tight Binding Linear Muffin Tin Orbital (TBLMTO) and linear fixed based method was used to investigate the structural properties and stability of the ZB. The experimentally measured lattice parameter and band structure parameters for ZnTe have been are used TBLMTO calculations with the LDA approximation. It is shown ZnTe is direct band gap semiconductor material and its band gap value is 0.97 eV. The band gap was increased using LDA its band gap value is 1.12 eV. The DOS and PDOS graph showed that the result was with good agreement with experimental values. The band dispersion between the VB and CB was also discussed with the experimental values. The COHP figure showed the bonding states between the CB and VB along with the integrated CHOP values.
Fig 6: Partial Density of States (PDOS) ZnTe in the groundstates configurations. The Fermi level is set to zero. The Fig.6 it shows the partial DOS of ZnTe the top of the valence band is complete band whereas conduction bands is partially filled and empty bands. The top of the valence band contains s band of tellurium with 40 states/eV its means that contributions of electron for the conduction between the CB and VB is from the s band of tellurium. The d band for zinc and Te it's delocalized in the bottom of the valence band, it type of bands donâ€™t help to conduction of electrons, because its bottom of the valence bands.
REFERENCES
3.2.3. Crystal Orbital Hamiltonian Population (COHP) Another useful tool to distinguish bonding, antibonding, and nonbonding interaction between atoms is the crystal orbital population (COHP). According to this COHP concept negative COHP values indicate bonding, positive values antibonding, and zero COHP together with finite DOS value suggests nonbonding states. The COHP is a quite meaningful way to measure the effective strength of bond interactions. The calculated COHP for Zn and Te are displayed in Fig. 7. For both Zn and Te atoms the VB consists of bonding states and the CB of antibonding states indicating that both have strong bonding interaction with the both atoms. The integrated COHP value (it's provides a measure of bond strength) for 1.53
ÂŠ 2018, IRJET

Impact Factor value: 7.211

[1]
S.K. Gupta , S. Kumar, S. Auluck , Physica B 404 (2009), pp. 37893794.
[2]
Tawat Suriwong, Somchai Thongtem, Materials
[3]
Let. 63 (2009) pp. 21032106.
[4]
YanqinGai, GangTang Phy.Let. A 378(2014) pp. 8285.
[5]
E. Deligoz, K. Colakoglu, Y. Ciftci, Physica B 373 (2006), pp. 124 130.
[6]
R. Franco, P. MoriSanchez, and J. M. Recio, Phys. Rev B, 68 (2003), pp. 195208195213.
Thongtem,
ISO 9001:2008 Certified Journal

Titipun
Page 2660
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 07  July 2018
pISSN: 23950072
www.irjet.net
[7]
J. PellicerPorres, D. MartnezGarca, Ch. FerrerRoca, A. Segura, and V. MuozSanjos, Phys. Rev, B 71 (2005) pp. 035210035217.
[8]
A. Zaoui, M. Zaoui, S. Kacimi, A. Boukortt, B. Bouhafs, Materials Chemistry and Physics, 120 (2010), 98103.
[9]
Mandana Safaria, Zohreh Izadia, Jaafar Jalilian, Iftikhar Ahmad, Saeid JalaliAsadabadi, Phys. Let.(2017), Accepted Manuscript.
[10]
[11]
S. Ramasubramanian, R. Thangavel, M. Rajagopalan, J. Kumar, Journal of Alloys and Compounds 479 (2009), pp.414419. C. Stampfl and C. G. Van de Walle, Phy. Rev. B 59 (1999), pp. 5521 5536.
[12]
D. J. Chadi, Phy. Rev. Lett. 72 (1994) pp. 534.
[13]
F.Benosman, N. Benosman, S. Mecabioh, B. Abbar, B.Bouhafs, Computational Materials Science 93 (2014), pp.2228.
[14]
YanXiao Han, ChuanLu Yang, JunSheng Yang, MeiShanWang,XiaoGuang Ma, Physica B 417 (2013) pp. 1723.
[15]
N.A. Noor, S. Ali, G. Murtaza, M. Sajjad, S.M. AlayeAbbas, A. Shaukat, Alahmed, Reshak, Computational Materials Science 93(2014) pp. 151159.
[16]
Bal K. Agrawal, P. S. Yadav, and Savitri Agrawal, Phys. Rev. B 50,(2000) pp. 1488214889.
[17]
J. PellicerPorres, A. Segura, V. Munoz, and J. Zuniga, Phys. Rev. B, 65 (2001), pp. 012109012113.
[18]
M. M. Sigalas, Phys. Rev. B, 50 (1994), 72557262.
[19]
E. Engel and S. H. Vosko, Phys. Rev. B 47 (1993), pp. 1316413172.
[20]
L .Ley, R. A. Pollak, F. R. McFecly, S. p. Kowalczyk, and D. A. Shirley, Phys. Rev. B, 9 (1974), pp. 600622.
[21]
N. Bouarissa, S.A. Siddiqui, A. Hajry, S. Saib, M. Boucenna, Computational Materials Science 83(2014) pp.2226.
[22]
Ali Gltekin, MustafaKemalztrk, TunusBa, Materials Science in Processing 39 (2015) pp. 629635.
[23]
Jaafar Jalilian, Mandana Safari, Phy. Let. A 381 (2017) pp.13131320.
ÂŠ 2018, IRJET

[24]
S.Lalitha, S.Zh.Karazhanov, S.Senthilarasu,
P.Ravindran,
[25]
R.Sathyamoorthy and J.Janabergenov, Physica B, 387 (2007) pp. 227238.
[26]
W. Kohn and L.J. Sham: PRA. 140 (1965) pp. 1133.
[27]
W. Kohn, Rev.mod. Phys. 71 (1998) pp. 1253.
[28]
Ayoub Nassour, Computational Materials Science 77 (2013) pp. 403407.
[29]
M. P andiaraman, N. Soundararajan, C. Vijayan, J. Ovo. Phy. Rev.7 (2000) pp. 2127.
[30]
A.E. Merad, M.B. Kanoun, S. GoumriSaid, Journal of Magnetism and Magnetic Materials 302 (2006), pp. 536542.
[31]
M. Shobana and S. R. Meher, Journal of Alloys and Compounds (2018), Accepted Manuscript.
[32]
H. Rozale, A. Lazreg, A. Chahed, P. Ruteran, Superlattices and Microstructures 46 (2009), pp.554562.
[33]
C. Tablero, Computational Materials Science 49(2010) pp.368371.
MehmetTamer, Semiconductor
Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 2661
https://www.irjet.net/archives/V5/i7/IRJETV5I7469.pdf
Published on Sep 12, 2018
https://www.irjet.net/archives/V5/i7/IRJETV5I7469.pdf